The handle http://hdl.handle.net/1887/44732
olds various files of this Leiden University
: Torren, Alexander J.H. van der
: Growing oxide thin films in a low-energy electron microscope
Growing oxide thin films in a
Low-Energy Electron Microscope
ter verkrijging van
de graad van Doctor aan de Universiteit Leiden, op gezag van Rector Magnificus prof. mr. C.J.J.M. Stolker,
volgens besluit van het College voor Promoties te verdedigen op 5 december 2016
klokke 11:15 uur
Alexander Johannes Hendrikus van der Torren
Promotiecommissie: Prof. dr. R. Dittmann (Forschungszentrum J¨ulich / RWTH Aachen)
Prof. dr. A.J.H.M. Rijnders (Universiteit Twente)
Dr. A. Caviglia (Technische Universiteit Delft) Prof. dr. E. R. Eliel
Prof. dr. ir. T.H. Oosterkamp
Casimir PhD series, Delft-Leiden 2016-32 ISBN 978-90-8593-276-5
An electronic version of this thesis can be found at
The work described in this thesis is supported by the Netherlands Organisation for Scientific Research (NWO) by means of a ”NWO Groot” grant and by the Leiden-Delft Consortium NanoFront.
The work is part of the research programmes NWOnano and DESCO, administered by the Foundation for Fundamental Research on Matter (FOM), which is part of NWO.
1 Introduction 1
1.1 Introduction . . . 1
1.2 Thesis outline . . . 2
References . . . 4
2 The LaAlO3/SrTiO3 interface 5 2.1 Transition-metal oxides . . . 6
2.2 The LaAlO3/SrTiO3Interface . . . 8
2.3 Oxygen vacancies . . . 10
2.4 Stoichiometry . . . 11
References . . . 12
3 Low-Energy Electron Microscopy (LEEM) 15 3.1 Introduction to LEEM . . . 16
3.2 Aberration-corrected LEEM . . . 17
3.3 Standard imaging techniques . . . 18
3.3.1 Low-energy electron diffraction (LEED) . . . 18
3.3.2 Bright field & dark field LEEM andµLEED . . . 19
3.3.3 LEEM-IV . . . 20
3.3.4 Photoemission electron microscopy (PEEM) . . . 20
3.4 Extending the possibilities . . . 20
3.4.1 Hardware . . . 20
3.4.2 Software . . . 21
3.4.3 Spot-profile-analysis LEED (SPA-LEED) . . . 22
3.4.4 Angle-resolved reflection electron spectroscopy (ARRES) . . 24
References . . . 25
4 Formation of a mixed ordered termination on the surface of LaAlO3(001) 27 4.1 Introduction . . . 29
4.2 Experimental . . . 30
4.3 Results . . . 32
4.3.1 Reconstructed surfaces . . . 32
4.3.2 The singly terminated surface . . . 35
4.3.3 On the formation of the mixed ordered termination . . . 36
4.4 Discussion . . . 37
4.5 Summary . . . 39
5 Imaging pulsed laser deposition growth of homo-epitaxial
SrTiO3 by Low-Energy Electron Microscopy 43
5.1 Introduction . . . 45
5.2 Experimental . . . 45
5.2.1 LEEM . . . 45
5.2.2 In-situ pulsed laser deposition . . . 46
5.2.3 LEEM extensions . . . 47
5.2.4 Sample preparation . . . 48
5.3 Results and discussion . . . 48
5.3.1 Following the growth . . . 49
5.3.2 Real space . . . 50
5.3.3 Spot-profile-analysis low-energy electron diffraction . . . 51
5.3.4 Angle-resolved reflection electron spectroscopy . . . 55
5.4 Conclusion . . . 56
References . . . 58
6 Finding signatures of the conducting LaAlO3/SrTiO3 interface at the growth temperature by electron reflection 61 6.1 Introduction . . . 63
6.2 Experimental setup and sample preparation . . . 64
6.3 Results . . . 64
6.4 Discussion . . . 70
6.5 Summary . . . 72
6.6 Appendix . . . 73
References . . . 74
7 Growing a LaAlO3/SrTiO3 heterostructure on Ca2Nb3O10 nanosheets 77 7.1 Introduction . . . 79
7.2 Experimental . . . 79
7.3 Results . . . 80
7.4 Discussion . . . 87
7.5 Summary . . . 89
References . . . 90
Curriculum Vitae 101
List of publications 103
Silicon is the workhorse for modern electronics. The performance of Si-based de-vices is mainly boosted by their miniaturization, which will soon be limited by quantum mechanical obstacles. A way to overcome this is to find other materi-als than the covalent semiconductors, that can be used in electronics. Silicon is a conventional semiconductor where the conductance or metallicity derives from exciting electrons over the band gap, or doping the material with either electrons or holes. In all cases, the number of charge carriers is low, with in particular long screening lengths for electric fields as a consequence. In silicon, the charge carriers behave as independent particles, with little interaction between them selves or with the lattice. In contrast, in transition metal oxides (TMO) the metallicity is deter-mined by details of the electron-electron interaction between the 3d electrons of the transition metal ion. The carrier concentration can be very high, in the order of an electron per atom, and screening lengths small. Also, the interactions can lead to complex phenomena such as high-temperature superconductivity or colos-sal magnetoresistance. Special properties and phenomena can also be achieved at the interface between different oxides. As Herbert Kroemer said during his Nobel lecture: ”Often, it may be said that the interface is the device”1. Already many
devices based on conventional semiconductors exploit interfaces, for example tran-sistors, lasers, memory and solar cells. The interfaces between TMOs, however open up a new world of interesting physics.
ability to obtain well-defined interfaces by fabricating surfaces consisting of only a single well-defined ionic or atomic plane, the so-called singly-terminated surface, has been a key step to obtain sharp interfaces2. Furthermore, the ability to grow
clean multilayers by molecular-beam epitaxy (MBE)3, and pulsed laser deposition
(PLD)4 has been of utmost importance. Moreover, the development of in-situ
reflection high-energy electron diffraction (RHEED)5for PLD at elevated pressures has led to thickness control down to the unit cell range.
To further optimize the material properties more information during the growth process would be of great value. Especially the structural and electronic prop-erties are important for the resulting film. Basic structural information can be obtained from the diffraction pattern obtained by RHEED but, electronic infor-mation is mostly missing. Other analysis techniques have been hampered by the extreme conditions, i.e. high temperature and oxygen background pressures. The requirements of surface sensitivity and non-invasive, non-contact techniques limit the analysis to electron optical techniques.
As most widely used system to grow TMOs we focus on PLD. We extend the possibility for in-situ film growth analysis by introducing low-energy electron microscopy (LEEM), with in-situ PLD system, as a new technique in this field. RHEED does not allow for spatial resolution and is more difficult to analyze than low-energy electron diffraction (LEED). Low-energy electron microscopy (LEEM) is able to combine spatial resolution with LEED. New developments, partially in our lab, allow one to investigate the electronic structure of a surface or thin film6.
This extends LEEM to a versatile set-up for material science, combining structural and electronic properties with lateral resolution and fast investigation.
An ideal device for electronics would be a two dimensional electron gas (2-DEG) at the interface between two insulators, with high electron mobility, tunable by a gate and working at room temperature. The 2-DEG found between the TMO band-insulators LaAlO3and SrTiO3 was a remarkable discovery7, which comes close to
this ideal device. However, the exact origin of this 2-DEG is still not understood. In this thesis we will use LEEM as a method to investigate the film properties of the hetero-structure during growth.
The main material system to be investigated is the LaAlO3/SrTiO3interface. This
will be introduced in chapter 2 and the method used for studying the interface, LEEM with its full set of subtechniques, in chapter 3. While the SrTiO3
build-ing block has already been studied in LEEM by Hesselberth et al.8 we continue
with the other building block, LaAlO3, in chapter 4. For the growth studies we
require a PLD system. Its development is described in chapter 5. Also its abili-ties are demonstrated by the growth of homoepitaxial SrTiO3. With the building
blocks and equipment in place we study the formation of the LaAlO3/SrTiO3
hetero-structure in chapter 6. Finally, we use our knowledge about the LaAlO3/
11.2. Thesis outline
 H. Kroemer,Nobel Lecture: Quasielectric fields and band offsets: teaching elec-trons new tricks, Reviews of Modern Physics 73, 783 (2001).
 M. Kawasaki, K. Takahashi, T. Maeda, R. Tsuchiya, M. Shinohara, O. Ishiyama, T. Yonezawa, M. Yoshimoto, and H. Koinuma,Atomic Control of the SrTiO3 Crystal Surface, Science 266, 1540 (1994).
 D. G. Schlom, J. N. Eckstein, E. S. Hellman, S. K. Streiffer, J. S. H. Jr, M. R. Beasley, J. C. Bravman, T. H. Geballe, C. Webb, K. E. v. Dessonneck, and F. Turner, Molecular beam epitaxy of layered DyBaCuO compounds, Applied Physics Letters53, 1660 (1988).
 D. Dijkkamp, T. Venkatesan, X. D. Wu, S. A. Shaheen, N. Jisrawi, Y. H. Min-Lee, W. L. McLean, and M. Croft,Preparation of YBaCu oxide superconductor thin films using pulsed laser evaporation from high Tc bulk material, Applied Physics Letters51, 619 (1987).
 G. J. H. M. Rijnders, G. Koster, D. H. A. Blank, and H. Rogalla, In situ monitoring during pulsed laser deposition of complex oxides using reflection high energy electron diffraction under high oxygen pressure, Applied Physics Letters70, 1888 (1997).
 J. Jobst, J. Kautz, D. Geelen, R. M. Tromp, and S. J. van der Molen,Nanoscale measurements of unoccupied band dispersion in few-layer graphene, Nature Communications6, 8926 (2015).
 A. Ohtomo and H. Y. Hwang, A high-mobility electron gas at the LaAlO3/SrTiO3 heterointerface, Nature427, 423 (2004).
 M. B. S. Hesselberth, S. J. v. d. Molen, and J. Aarts,The surface structure of SrTiO3at high temperatures under influence of oxygen, Applied Physics Letters
LaAlO3and SrTiO3 are cubic perovskites and wide band gap insulators which differ
in one aspect: SrTiO3 is a non-polar material, where each layer stacked along a
principal axis of the cube is change-neutral. LaAlO3 is polar, with layers having
Transition metal oxides (TMO’s) show many exciting phenomena compared to sim-ple covalent semiconductors. Strong Coulomb repulsion between the 3d electrons of the TM ion, parametrized byU, tend to localize them on the atoms, leading to an insulating state. The energy gap to the conducting states is roughly determined by U −2zt, where t is the site-to-site transfer integral of the d-electrons, and z
is the number of nearest neighbors. Ift << U, as is often the case, this leads to the so-called Mott-insulating state. Such an insulator is very different from cova-lent semiconductors such as Si, and GaAs, where the four hybridized sp3 electrons
form shared pairs with four nearest neighbor atoms. The electrons localize between the atoms, as a result of the competition between electron-nucleus attraction and electron-electron repulsion. The Mott state is charge-ordered, but the subtle in-terplay between charge, spin, and lattice structure also leads to spin and orbital order. Figure 2.1a and b show the doping phase diagrams of La1-xSrxMnO3 and
0.0 0.1 0.2 0.3 0.4 0.5 0.6 x 0 100 200 300 400 Temperature (K) CI FI FM AFM PI PI a
0.0 0.1 0.2 0.3 0.4 x 0 20 40 60 80 100 Temperature (K) Antiferromagnet Mott-insulator Pseudo-gap Fermi liquid Superconducting Non-Fermi liquid b
Figure 2.1: Phase diagram of (a) La1-xSrxMnO3, based on data from Ref.1–3. PM, PI, FM,
AFM, FI, and CI denote, paramagnetic metal, paramagnetic insulator, ferromagnetic metal, anti-ferromagnetic metal, anti-ferromagnetic insulator, and spin-canted insulator states, respectively. (b) La2-xSrxCuO4, based on data from Ref.4.
La2-xSrxCuO4, respectively. In (La,Sr)MnO3 the Sr2+ ion dopes holes into the
MnO2 complex, leading to a mix of Mn3+ and Mn4+ valencies. The latter results
in a hole in the d-band and (at low temperatures) a change from an antiferro-magnetic canted insulator (CI in Fig. 2.1a) to a ferroantiferro-magnetic metal (FM). This state becomes paramagnetic insulating at higher temperatures, resulting in the well-known colossal magnetoresistance effect. In (La,Sr2)CuO4 the doping leads
to even more dramatic effects. Doping holes into the CuO2 complexes now yields
22.1. Transition-metal oxides
The effective masses of charge carriers in TMOs are an order of magnitude higher than in semiconductors, which is partly due to the strong coupling with the lattice and the reorientation possibilities for the oxygen octahedra. Together with high carrier concentrations this leads to short screening lengths for electric fields, in the order of 1 to 100 nm.
Figure 2.2:Unit cells of the perovskite structure with the ABO3chemical formula. Here A is in
green (corner), B in blue (center) and O in red (cube faces). Furthermore, the AO plane is shown in green and the BO2plane in blue.
A much studied structure of TMOs is the cubic perovskite structure (Fig. 2.2). The chemical structure is ABO3. Here the A is an alkaline earth metal or a rare
earth metal and the B is a transition metal or a metalloid. Under pressure and tem-perature the structure can change from cubic to orthorhombic, tetragonal, rhombo-hedral or monoclinic. Along the (001) direction the structure can be seen as, built up from AO and BO2 planes, indicated with blue and green planes in figure 2.2.
In this thesis I will focus on the 2-dimensional electron gas between the TMOs SrTiO3and LaAlO3. Strictly speaking, SrTiO3is a TMO, but not a Mott-insulator,
the Ti4+has an empty d-shell. However, doping can fill the Ti d-shell in the SrTiO 3,
showing TMO physics. Moreover, LaAlO3 is not strictly a TMO, since Al is not a
transition metal, but structure and physics is close to the one of the TMOs and it is in general seen as part of the group. SrTiO3 and LaAlO3 are both perovskites
and insulators with bandgaps of 3.2 eV5 and 5.6 eV6 respectively. Their lattice
constants (STO: 3.905 ˚A7, LAO: 3.789 ˚A8) have only a small mismatch of 3 %,
resulting in epitaxial growth when stacking the two materials. Both materials are widely used as substrates, and are easily commercially available as single crystals. As-received crystals have a mixed terminated surface with both areas with AO and BO2 planes. For SrTiO3 the termination can chemically be changed to TiO29,10,
SrO on a TiO2 terminated surface. For LaAlO3 the termination is more complex
and it will be discussed in chapter 4.
At the interface of LaAlO3 and SrTiO3 a conducting interface is found. This is
a different interface than in covalent semiconductors. Where for instance at the
Figure 2.3: Comparison between the 2-DEG at the GaAs/AlxGa1−xAs interface (top) and the
2-DEL at the LaAlO3/SrTiO3 interface (bottom). Taken from Ref.11.
interface of the covalent semiconductors GaAs/AlxGa1−xAs the mobile carriers
move into two-dimensional subbands within the quantum well generated by band bending, at the LaAlO3/SrTiO3interface multiple quantum wells are found given
by the ionic potentials of the TiO6octahedra (see fig. 2.3). The electrons are subject
to the correlations of the Ti 3d bands and form an two dimensional electron liquid (2-DEL) rather than a gas12. This electron liquid is strongly confined, which is very
advantageous for screening and switching applications as well as for miniaturization of devices. For historic reasons we will often still use 2-DEG instead of 2-DEL.
The interface can actually be made in two different configurations. First, when the SrTiO3 is TiO2 terminated, growing epitaxial LaAlO3 results in a TiO2/LaO
interface, which can become conducting. Second, when the terminating layer is SrO the interface will be SrO/AlO2. This interface turns out to be insulating13,14.
For the conducting interface, Thiel et al.15 found that the surface only becomes
conducting when the LaAlO3layer consists of four or more unit cells. One and two
22.2. The LaAlO3/SrTiO3 Interface
e/2 e/2 e/2 e/2 e/2 e/2 e/2 e/2 e/2 1– 1+ 1– 1+ 1– 1– 1+ 1+ 0 0 0 0 0 0 Al3+O24–
1+ 1+ 1– 1– 0 0 0 0 1– 1– 1+ 1+ 0 0 0 0
ρ E V ρ E V
ρ E V ρ E V
1/2– 1/2+ 1.5– a b c d
Figure 2.4: Illustration of the polar catastrophe model in the LaAlO3/SrTiO3 hetero-structure.
The stacking sequence of LaAlO3and SrTiO3layers is shown with their oxidation levels and final
net charge per layer. In the diagramsρis the net charge per layer,Ethe resulting electric field andV the potential buildup. a and b illustrate the potential buildup for a n-type (TiO2/LaO) and
p-type (SrO/AlO2) interface respectively, leading to a diverging potential. In c half an electron
charge is transferred from the surface to the interface to avoid the divergence. For the p-type interface, one would expect the electron is transferred from the interface to the surface. However, an energetically more favorable structural reconstruction16appears. Image from Ref.14.
To understand this remarkable effect of a 2-dimensional electron gas between two insulators, the role of the SrTiO3and LaAlO3layers are now further discussed.
These building blocks can be described as stacked AO and BO2layers as stated
ear-lier. Writing down these layers and their charges we find for the SrTiO3, Sr2+O2−
2 , both having zero net charge. In contrast, for LaAlO3 the layers
are La3+O2− and Al3+O42−, respectively positive and negatively charged. This is illustrated in figure 2.4. The charged layers in the LaAlO3 can be seen as parallel
plate capacitors with a charge ρ, resulting in an electric field E between them, which results in a potential buildupV. Starting from a neutral SrTiO3 layer the
potential builds up without bound, as the thickness of LaAlO3 grows (Fig. 2.4a),
which is not physically possible. This can be solved by an electronic or structural reconstruction. In the case of an electronic reconstruction, half an electron is trans-ferred from the LaAlO3surface towards the interface (Fig. 2.4c), resulting in half a
free electron per unit cell at the interface creating half the charge at the interface. This is the so called polar catastrophe13,14model. This potential buildup fits
rea-sonably well with the transition from insulating to conducting interface at three to four unit cells. Only for four unit cells and more the potential buildup is strong enough for the electron transfer to take place.
The resulting electrons at the interface will change the Ti4+ to Ti3+. In that
case, we call it a n-type interface. On the other hand if the SrTiO3surface is SrO
to be transferred away from the interface to the LaAlO3 surface (Fig. 2.4d). This
would result in a p-type interface as an electron has to be removed from the O-2p band. This is energetically more expensive and a structural reconstruction is more favorable16 resulting in an insulating interface.
Although this model presents a good description of the conducting interface, it cannot be the full story. In particular core-level X-ray photoemission spectroscopy (XPS) measurements have not been able to measure the potential buildup17,18.
Furthermore, there is strong evidence for an important role of defects and stoi-chiometry, which now will be discussed.
10 100 10–2 10–1 100 101 102 103 104 105
Temperature (K) S he et r es is ta nc e ( Ω pe r )
Figure 2.5:Sheet resistance as function of temperature of the LaAlO3/SrTiO3interface
depend-ing on oxygen background pressure durdepend-ing growth as indicated in the figure. Note the minimum who occurs for pressures above 10−4mbar. Taken from Ref.19.
The number of oxygen vacancies is mainly influenced by the oxygen background pressure during growth and is well described by Brinkmanet al.19. Figure 2.5
sum-marizes the salient behavior of the sheet resistance of the interface as function of temperature for different values of the oxygen background pressure during growth. At pressures of 1×10−6 mbar and lower the amount of oxygen in the SrTiO
regime different types of physics are found at the interface, such as superconduc-tivity20–22 and magnetism19,23–25. The minimum occurring at pressures above
1×10−4 mbar is often connected to the presence of some kind of magnetism.
To stay clearly away from bulk conductivity, but preserve UHV conditions in our low-energy electron microscope without taking extra precautions, we decided to use a background pressure of 5×10−5mbar O2 in the experiments involving the
It has been found that also the stoichiometry of the deposited LaAlO3-layer is
of crucial importance for rendering the interface conducting or insulating26–29.
Warusawithanaet al.27using molecular beam epitaxy (MBE), found that the La/Al
ratio has to be smaller than 0.97 to obtain a conducting interface. Breckenfeld
et al.30, using PLD, found that at 2 K the interface sheet resistances using 4 %
La-deficient LaAlO3 is almost ten orders of magnitude lower than the interface sheet
resistance using 5 % La-excess LaAlO3. Also, Dildar et al.26 found that LaAlO3
deposited on SrTiO3 by sputtering in 1 mbar of oxygen showed a La-excess of
7 %, while the interface was insulating. This stoichiometry dependence emphasizes the importance of defects in the SrTiO3 and LaAlO3 during the formation of the
interface conductance. In particular, it has been pointed out that excess Al can substitute on the La-sites, while La excess leads to Al2O3-vacancy complexes27,
with significant differences in the way the charge distribution problem can be solved. However, how this exactly leads to either a conducting or a non-conducting interface is not yet fully understood.
The stoichiometry issue is the more important since it is strongly influenced by the growth conditions. Growth of LaAlO3/SrTiO3interfaces is most frequently
performed by pulsed laser deposition (PLD), the primary work horse for complex oxide growth. Apart from the fact that PLD is a relative cheap option compared to MBE, it was long believed that PLD was a technique which would transfer a ma-terial preserving the stoichiometry. However, also PLD is a complex process where laser fluence and background pressure play an important role in the stoichiometry of the film. Here the ablation efficiency of the ions and the scattering processes between ions and the background gas play an important role31. In these scattering
 E. Dagotto, T. Hotta, and A. Moreo,Colossal magnetoresistant materials: the key role of phase separation, Physics Reports344, 1 (2001).
 A. Urushibara, Y. Moritomo, T. Arima, A. Asamitsu, G. Kido, and Y. Tokura,
Insulator-metal transition and giant magnetoresistance in La1−xSrxMnO3,
Physical Review B51, 14103 (1995).
 H. Fujishiro, M. Ikebe, and Y. Konno, Phase Transition to Antiferromagnetic State in La1−XSrXMnO3 (X0.5), Journal of the Physical Society of Japan67,
 M. P. M. Dean, G. Dellea, R. S. Springell, F. Yakhou-Harris, K. Kummer, N. B. Brookes, X. Liu, Y.-J. Sun, J. Strle, T. Schmitt, L. Braicovich, G. Ghiringhelli, I. Boovi, and J. P. Hill, Persistence of magnetic excitations in La2xSrxCuO4
from the undoped insulator to the heavily overdoped non-superconducting metal, Nature Materials12, 1019 (2013).
 H. Weakliem, W. Burke, and V. Korsun, Optical Properties of SrTiO3 and
LiNbO3, R.C.A. Review36, 149 (1975).
 S.-G. Lim, S. Kriventsov, T. N. Jackson, J. H. Haeni, D. G. Schlom, A. M. Bal-bashov, R. Uecker, P. Reiche, J. L. Freeouf, and G. Lucovsky,Dielectric func-tions and optical bandgaps of high-K dielectrics for metal-oxide-semiconductor field-effect transistors by far ultraviolet spectroscopic ellipsometry, Journal of Applied Physics91, 4500 (2002).
 J. G. Bednorz and H. J. Scheel, Flame-fusion growth of SrTiO3, Journal of
Crystal Growth41, 5 (1977).
 S. Geller and V. B. Bala,Crystallographic studies of perovskite-like compounds. II. Rare earth alluminates, Acta Crystallographica9, 1019 (1956).
 M. Kawasaki, K. Takahashi, T. Maeda, R. Tsuchiya, M. Shinohara, O. Ishiyama, T. Yonezawa, M. Yoshimoto, and H. Koinuma,Atomic Control of the SrTiO3 Crystal Surface, Science 266, 1540 (1994).
 G. Koster, B. L. Kropman, G. J. H. M. Rijnders, D. H. A. Blank, and H. Ro-galla,Quasi-ideal strontium titanate crystal surfaces through formation of stron-tium hydroxide, Applied Physics Letters73, 2920 (1998).
 J. Mannhart and D. G. Schlom, Oxide Interfaces–An Opportunity for Elec-tronics, Science 327, 1607 (2010).
 M. Breitschaft, V. Tinkl, N. Pavlenko, S. Paetel, C. Richter, J. R. Kirtley, Y. C. Liao, G. Hammerl, V. Eyert, T. Kopp, and J. Mannhart,Two-dimensional elec-tron liquid state at LaAlO3-SrTiO3 interfaces, Physical Review B 81, 153414
 A. Ohtomo and H. Y. Hwang, A high-mobility electron gas at the LaAlO3/SrTiO3 heterointerface, Nature427, 423 (2004).
 N. Nakagawa, H. Y. Hwang, and D. A. Muller,Why some interfaces cannot be sharp, Nature Materials5, 204 (2006).
 S. Thiel, G. Hammerl, A. Schmehl, C. W. Schneider, and J. Mannhart, Tun-able Quasi-Two-Dimensional Electron Gases in Oxide Heterostructures, Science
313, 1942 (2006).
 L. Zhang, X.-F. Zhou, H.-T. Wang, J.-J. Xu, J. Li, E. G. Wang, and S.-H. Wei, Origin of insulating behavior of the p-type LaAlO3/SrTiO3 interface:
Polarization-induced asymmetric distribution of oxygen vacancies, Physical Re-view B82, 125412 (2010).
 Y. Segal, J. H. Ngai, J. W. Reiner, F. J. Walker, and C. H. Ahn,X-ray photoe-mission studies of the metal-insulator transition in LaAlO3/SrTiO3 structures
grown by molecular beam epitaxy, Physical Review B80, 241107 (2009).  M. Takizawa, S. Tsuda, T. Susaki, H. Y. Hwang, and A. Fujimori,Electronic
charges and electric potential at LaAlO3/SrTiO3interfaces studied by core-level
photoemission spectroscopy, Physical Review B84, 245124 (2011).
 A. Brinkman, M. Huijben, M. van Zalk, J. Huijben, U. Zeitler, J. C. Maan, W. G. van der Wiel, G. Rijnders, D. H. A. Blank, and H. Hilgenkamp,Magnetic effects at the interface between non-magnetic oxides, Nature Materials 6, 493 (2007).
 N. Reyren, S. Thiel, A. D. Caviglia, L. F. Kourkoutis, G. Hammerl, C. Richter, C. W. Schneider, T. Kopp, A.-S. Ruetschi, D. Jaccard, M. Gabay, D. A. Muller, J.-M. Triscone, and J. Mannhart,Superconducting Interfaces Between Insulat-ing Oxides, Science317, 1196 (2007).
 A. Joshua, S. Pecker, J. Ruhman, E. Altman, and S. Ilani,A universal critical density underlying the physics of electrons at the LaAlO3/SrTiO3 interface,
Nature Communications3, 1129 (2012).
 A. D. Caviglia, S. Gariglio, N. Reyren, D. Jaccard, T. Schneider, M. Gabay, S. Thiel, G. Hammerl, J. Mannhart, and J.-M. Triscone,Electric field control of the LaAlO3/SrTiO3 interface ground state, Nature456, 624 (2008).
 Ariando, X. Wang, G. Baskaran, Z. Q. Liu, J. Huijben, J. B. Yi, A. Annadi, A. R. Barman, A. Rusydi, S. Dhar, Y. P. Feng, J. Ding, H. Hilgenkamp, and T. Venkatesan, Electronic phase separation at the LaAlO3/SrTiO3 interface,
Nature Communications2, 188 (2011).
 J. A. Bert, B. Kalisky, C. Bell, M. Kim, Y. Hikita, H. Y. Hwang, and K. A. Moler, Direct imaging of the coexistence of ferromagnetism and superconduc-tivity at the LaAlO3/SrTiO3 interface, Nature Physics7, 767 (2011).
 I. M. Dildar, D. B. Boltje, M. H. S. Hesselberth, J. Aarts, Q. Xu, H. W. Zandbergen, and S. Harkema, Non-conducting interfaces of LaAlO3/SrTiO3
produced in sputter deposition: The role of stoichiometry, Applied Physics Let-ters102, 121601 (2013).
 M. P. Warusawithana, C. Richter, J. A. Mundy, P. Roy, J. Ludwig, S. Paetel, T. Heeg, A. A. Pawlicki, L. F. Kourkoutis, M. Zheng, M. Lee, B. Mulcahy, W. Zander, Y. Zhu, J. Schubert, J. N. Eckstein, D. A. Muller, C. S. Hellberg, J. Mannhart, and D. G. Schlom,LaAlO3stoichiometry is key to electron liquid
formation at LaAlO3/SrTiO3 interfaces, Nature Communications4(2013).
 H. K. Sato, C. Bell, Y. Hikita, and H. Y. Hwang,Stoichiometry control of the electronic properties of the LaAlO3/SrTiO3 heterointerface, Applied Physics
Letters102, 251602 (2013).
 E. Breckenfeld, R. Wilson, J. Karthik, A. R. Damodaran, D. G. Cahill, and L. W. Martin,Effect of Growth Induced (Non)Stoichiometry on the Structure, Dielectric Response, and Thermal Conductivity of SrTiO3 Thin Films,
Chem-istry of Materials24, 331 (2012).
 E. Breckenfeld, N. Bronn, J. Karthik, A. R. Damodaran, S. Lee, N. Mason, and L. W. Martin,Effect of Growth Induced (Non)Stoichiometry on Interfacial Conductance inLaAlO3/SrTiO3, Physical Review Letters110, 196804 (2013).
abberation corrector S1/D1/GL
TL OL OS
M1 M2 MPA1
ﬁeld ray aperture
Figure 3.1: Schematic view of the electron-optical system of a LEEM. The yellow part is only
included in the aberration corrected version. All electron-optical elements like lenses, deflectors and stigmators are labeled, and explained in the text.
Introduction to LEEM
Low-energy electron microscopy uses electrons up to 100 eV to perform surface sensitive imaging and spectroscopy. These low-energy electrons are very surface sensitive due to their low inelastic mean free path, which limits their penetration depth and is in the order of a few atomic layers1.
Unlike scanning electron microscopes (SEM), LEEM illuminates the entire field of view at once. This allows for real-time imaging of dynamic processes. Two im-portant components of a LEEM, are the magnetic prism array (MPA) and cathode objective lens. The MPA allows for transfer of the full field of view to the detector by separating the incoming, illuminating electrons from back-scattered electrons, used to form an image. The cathode lens is the crucial part for the low energy electrons as will be discussed later on. An illustration of the setup is shown in figure 3.1. First I will explain the non-aberration corrected version, in which the yellow part in figure 3.1 is absent.
33.2. Aberration-corrected LEEM
electron lenses. The electrons are focused by the gun lens (GL) and condenser lens (CL) and can be steered by a set of deflectors (D1-D3) before entering the magnetic prism array (MPA1), which bends the electrons by 90◦towards the sample. After passing the transfer lens (TL) the electrons arrive at the objective lens (OL). The objective lens consists of a magnetic lens and an electrostatic lens of which the sample forms the cathode. The sample is biased with a tunable negative high voltage close to the electron gun potential of 15 kV. The strong electric field (≈
10 kV/mm) decelerates the electrons to a selected energy in the range of 0 - 100 eV. An energy of 0 eV is called mirror mode, because the electrons just start to turn around before any interaction happened, and the sample becomes a mirror. After interaction with the sample, the electrons will be accelerated back to 15 keV in the same electric field. A diffraction pattern or in general the angular distribution of the electrons, is formed at the back focal plane of the objective lens and further along, a real-space image is formed at the image plane in the center of the magnetic prism array. To clarify the optical path, the field (blue) and axial (red) rays are drawn into figure 3.1. The axial or marginal ray starts at the point where the object crosses the optical axis and ends at the aperture stop. This ray crosses the optical axis at all points where an image is made. The field ray is parallel to the optical axis at the object and crosses the optical axis at the back focal plane.
Once the electrons are back at the prism array MPA1, it deflects the electrons downwards into the projector column. The projector column with lenses P1-4, mag-nifies and transfers the image onto the detector. Fast switching between imaging and diffraction mode is possible by turning on lens (P2) in the projector column. The lenses P4A-B can be used as a rotation free doublet for low magnifications or as a telescope for very strong magnification. The detector is build up out of a micro-channel plate, phosphor screen and camera. The channel plate amplifies the signal my multiplying the incoming electrons. The outgoing electrons are converted to photons with a phosphor screen, the photons are detected by a camera.
The ESCHER (Electronic, Structural and CHEmical nanoimaging in Real-time) machine is the LEEM system located at Leiden University. It is based on the aberration corrected FE-LEEM P90 instrument (SPECS GmbH, Berlin) designed by Tromp2,3. The advantage of an aberration corrected LEEM is an increased
spatial resolution up to 1.4 nm, a world record for LEEM, which was measured on this machine. The resolution of a LEEM machine is limited by the chromatic and spherical aberrations induced by the cathode objective lens OL. While these aberrations cannot be corrected by lenses since electron lenses can only be convex, the lowest order aberrations can be corrected by an electrostatic mirror4. The
Figure 3.2: a) A LEED pattern of mixed terminated SrTiO3 sample, taken at 14 eV. On the
edge the four bright diffraction spots of the cubic perovskite unit cell can be seen while the spots around the center are from two rotations of the√13×√13 R33.7 surface reconstruction. The spots of the 2×2 surface reconstruction are very vague. b) A multi darkfield image taken at 12 eV, red and green are the two rotations of the√13×√13 R33.7 surface reconstruction while the blue area is 2×2 reconstructed. c) A bright field image taken at 12 eV of the same sample. The 2×2 reconstructed area is dark. Also the step edges are dark, due to destructive interference or phase contrast.
by introducing a second magnetic prism array (MPA2, Fig. 3.1). An electrostatic transfer lens (ETL) is placed between the two prisms to invert the image without rotations such that the dispersion of the two prisms cancel. An extra set of lenses (M1/M2) is placed between MPA2 and mirror to create a rotation-free defocused image on the mirror, optimizing the mirror performance.
Standard imaging techniques
A low energy electron microscope offers a unique opportunity in sample analysis by combining many measurement techniques. In the following sections I will briefly describe the main techniques used.
Low-energy electron diffraction (LEED)
The driving force behind many of the imaging techniques ina LEEM is the oppor-tunity to combine real-space imaging with diffraction experiments. For electrons, crystalline samples will act as a grating and a diffraction pattern in the far field is the result. This technique is called low-energy electron diffraction (LEED) An example is shown in figure 3.2a of a SrTiO3 crystal annealed at 1200◦C in air for
12 hours. The annealing leads to a mixed terminated surface with areas of TiO2
and SrO areas5,6. On the edge of the image, bright spots are seen in a square
pat-tern, the square surface net of SrTiO3. In the center the specular spot represents
the electrons scattered back perpendicular to the surface. The other spots are a combination of a√13×√13 R33.7 surface reconstruction, with different directions, and a 2×2 reconstruction. The√13×√13 R33.7 surface reconstruction is known to exists on the TiO2 terminated part7. The 2×2 reconstruction is likely to be
33.3. Standard imaging techniques
Figure 3.3: µLEED images of a mixed terminated SrTiO3 sample. a) Taken at the 2×2
reconstructed part, blue in figure 3.2b. b) One of the two rotations of the√13×√13 R33.7 reconstructed part. Both images are taken at 14 eV.
Bright field & dark field LEEM and
As stated earlier the strength of LEEM is combining real-space and diffraction information. By placing an aperture around one of the diffraction spots, the ar-eas contributing to this spot can be imaged in real-space. An example is shown in figure 3.2b where three images are merged by adding them in red, green and blue. For every color in the image a diffraction spot of one of the three surface reconstructions is selected. The spots of the two rotations of the√13×√13 R33.7 reconstruction are selected for red and green while a spot of the 2×2 reconstruc-tion is selected for blue. In the results we can clearly see the diffracreconstruc-tion patterns originate from distinct areas of the surface.
One can also select the center or specular diffraction spot. The real-space image now shows contributions of two effects. In the first place the intensity at a given energy is related to the (electronic) structure as will be described in more detail in section 3.4.4. This can be observed in figure 3.2c, where the intensity is different on the TiO2 and SrO terminated areas. A second effect originates from the wave
nature of the electrons. The electron waves can cause destructive interference at the step edges, for specific energies of the incoming electrons. This produces dark lines as shown in figure 3.2c and is called phase contrast.
Not only a part of the diffraction image can be selected, but also a part of a real-space image. The aperture now selects only a small region on the sample and the reconstruction on this region can be imaged. This is demonstrated in figure 3.3, where figure 3.3a is taken on a TiO2terminated area and figure 3.3b on
a SrO terminated area of the SrTiO3sample. This technique is called micro-LEED
More quantitative data can be obtained from a diffraction pattern by not only collecting the position of the diffraction spots, but also the intensity dependence on the landing energy (or sample voltage) of the electrons. These are so called LEED-IV curves and can be used as a fingerprint or be compared with calculations of a model system. Compared to standard LEED the energies used in LEEM are even lower. This is sometimes called very low energy electron diffraction or VLEED. In this range multiple scattering is less important and for the specular diffraction spot, the data are close to the unoccupied band structure8,9. In LEEM this method can be extended with spatial resolution by selecting the specular diffraction spot with an aperture and image the real space IV-curve10.
Photoemission electron microscopy (PEEM)
By turning off the electron beam and illuminating the sample with UV light the machine can be changed to a photoemission electron microscope (PEEM). Although this is an interesting technique in itself, in this thesis it is mainly used for alignment and as a localization technique. The spot of the electron beam is around 5µm while the UV light illuminates the full sample so that images of a few hundred microns can be made.
Extending the possibilities
For the investigation of electronic and growth properties of perovskites like SrTiO3
and LaAlO3, a low-energy electron microscope is very suitable. It can perform
real-time imaging while allowing for the high measurement temperatures required for the growth of these oxide materials. However, many other components still had to be added. In the following section I will explain more about the exten-sions we developed for the study of perovskite growth. First of all, the hardware: pulsed laser deposition (PLD), preparation chamber, heating laser (including laser safety). However, these days a complex measurement machine cannot be controlled without software and long and repeatable growth experiments cannot be achieved without automation. To achieve the automation a flexible software system has been developed.
Furthermore, the layer-by-layer growth of the perovskites studied in this the-sis requires imaging techniques not commonly used in LEEM. Section 3.4.3 will introduce spot-profile analysis LEED (SPA-LEED). Improving the technique of angle-resolved reflection electron spectroscopy (ARRES) developed in our group allowed for repetitive probing of the electronic structure as will be explained in section 3.4.4.
33.4. Extending the possibilities
Figure 3.4: Example of data flow between software programs.
with a 100 W, 808 nm diode laser, the perovskite samples can be annealed in high oxygen pressures. This laser heater can also be attached to the main sample cham-ber to serve as an alternative for the electron bombardment heater. I developed a flexible interlock system enabling the heater to be used in combination with or next to the pulsed laser deposition system in both sample and preparation chamber while the machine is standing in an open experimental hall.
Long repeatable growth processes require logging of growth parameters during the process as well as automatic control of the equipment. For this, new software has been developed. Figure 3.4 shows a flow diagram of the software programs and the data flows between them.
The existing LEEM software consists of a database containing all the electron lens values. These values can be controlled from the software as well as via a network transparent protocol. The program has been changed to extend the com-munication protocol and to save the database to the header of every image in order to have a complete description of the ’machine state’ at the time the image was taken. Furthermore, the database can be extended with new variables via the communication protocol.
stability or the need to restart the LEEM control software. Figure 3.4 shows a program ’pressures’ which reads the pressure gauge and temperature and pushes it to LEEM software. The program writes to a log file to support plotting of temperature and pressure independent of imaging.
On the fly hardware changes are required when changing from standard LEEM to pulsed laser deposition (chapter 5) or other new developments like potentiome-try11 or eV-TEM12. For the hardware control the communication protocol is
ex-tended with a callback function. When the callback function is enabled, the LEEM software sends a signal to the python program when the variable is changed. The python software can then communicate the change to the hardware. Figure 3.4 also shows a ’Laser control’ program communicating back and forth to the hardware, and the LEEM software.
Once the basic protocols are in place, extra features can be added like a plotting script which can now communicate to our python server as well as directly to the LEEM software to plot for example the electron landing energy or sample temperature.
Measurement automation scripts can use the same protocol to communicate to LEEM software. For this purpose the communication protocol has been further extended. In the first place one would like to stop and test scripts without the risk of ending up in an unwanted machine state, where possibly the alignment of the microscope is lost. To accommodate this, variables have to be locked when a script it started. When a variable is locked, the value is stored and when the connection to the measurement script is lost, the value is restored to its original state. Moreover, collision between scripts is avoided by allowing only one script to change a variable.
Spot-profile-analysis LEED (SPA-LEED)
Measurement automation allows for new measurement techniques. One of these techniques is spot-profile-analysis low-energy electron diffraction (SPA-LEED). In SPA-LEED we use the fact that the diffraction pattern yields more information than only the intensity and position of the diffraction spots, which results in crystal structure information. By analyzing the shape of the diffraction spots we can learn about the surface roughness. This is an important analysis for layer-by-layer growth, where the surface roughens when a layer starts to grow and flattens when a full layer has been grown.
An example is shown in figure 3.5 for the specular diffraction spot. Here fig-ure 3.5a shows the intensity versus energy (LEED-IV-curve) and figfig-ure 3.5b shows two example spot profiles at 40 eV (red) and 75 eV (green, dashed). This SPA-LEED technique is not so commonly used in combination with LEEM. An im-portant reason is the change in intensity of the reflected electrons in the order of 104 when scanning the energy as can be seen in figure 3.5a. This large range of
33.4. Extending the possibilities
0 20 40 60 80 100 120
−0.2 0.0 0.2
Figure 3.5: a) Maximum specular spot intensity versus energy for 1/2 unit cell homo-epitaxial
SrTiO3. b) Spot profile for the same sample at 40 eV (red) and 75 eV (green, dashed). Kkis the
in-plane wave vector of the electrons forming the diffraction spot.
To gain enough image depth for the images shown in figure 3.5, a method was developed to automatically adjust the gain of our imaging system, keeping the maximum intensity on the camera around 75% of its maximum. As described before, the imaging system here is a microchannel plate detector which multiplies the incoming electrons. The outgoing electrons are converted to photons with a phosphor screen, the photons are finally detected by the camera. The gain of the channel plates can easily be adopted by changing the amplification voltage. We characterized this gain to followI= (Icmr−b)e−GVcp, whereIcmr is the intensity
measured by the camera, b the background signal originating from the camera readout noise,Vcpis the voltage over the channel plates in kV,Gis the gain andI
is the final intensity. Here the gain was measured to be 20 kV−1. In practice the
channel plate voltageVcp lies between 0.9 kV and 1.7 kV resulting in a six orders
of magnitude amplification range.
For a so-called high-dynamic range energy scan, automatic adjustment of the gain is implemented in the energy scan script by calculating the gain required for 75% saturation of the camera after each image. This gain is used to capture the next frame. Expecting a smooth and slowly changing brightness, the intensity of the next image will thus lie within range of the camera.
Angle-resolved reflection electron spectroscopy
Parallel to my work Johannes Jobst and Jaap Kautz developed a technique to probe the unoccupied band structure of graphene9 in our LEEM setup. In this
technique the intensity of the specular spot is measured as function of the energy and in-plane momentum of the electrons. In first order the signal depends on the availability of a state in the material with the same energy and in-plane momentum
kkas the electron. If this state is available the electron will couple into the material,
otherwise it will reflect.
This measurement can be done in diffraction, where one averages the signal over a 5 micron spot, as well as in real-space where an aperture is used around the specular spot and full spatial resolution can be obtained. I improved this technique and made it easy to use for quick and repetitive measurements by adding high dynamic range as well as full automation of the measurement. For automation of real-space ARRES it is important to not only change the parallel momentumkkof
 S. Tanuma, C. J. Powell, and D. R. Penn, Calculations of electron inelastic mean free paths. V. Data for 14 organic compounds over the 502000 eV range, Surface and Interface Analysis21, 165 (1994).
 R. Tromp, J. Hannon, A. Ellis, W. Wan, A. Berghaus, and O. Schaff,A new aberration-corrected, energy-filtered LEEM/PEEM instrument. I. Principles and design, Ultramicroscopy110, 852 (2010).
 R. Tromp, J. Hannon, W. Wan, A. Berghaus, and O. Schaff,A new aberration-corrected, energy-filtered LEEM/PEEM instrument II. Operation and results, Ultramicroscopy (2013).
 S. M. Schramm, J. Kautz, A. Berghaus, O. Schaff, R. M. Tromp, and S. J. van der Molen, Low-energy electron microscopy and spectroscopy with ES-CHER: Status and prospects, IBM Journal of Research and Development55, 1:1 (2011).
 R. Bachelet, F. Snchez, F. J. Palomares, C. Ocal, and J. Fontcuberta, Atomi-cally flat SrO-terminated SrTiO3(001) substrate, Applied Physics Letters95,
 R. Bachelet, F. Snchez, J. Santiso, C. Munuera, C. Ocal, and J. Fontcuberta,
Self-Assembly of SrTiO3(001) Chemical-Terminations: A Route for
Oxide-Nanostructure Fabrication by Selective Growth, Chemistry of Materials 21, 2494 (2009).
 D. M. Kienzle, A. E. Becerra-Toledo, and L. D. Marks, Vacant-Site Octahe-dral Tilings on SrTiO3 (001), the (
13×√13)R33.7◦ Surface, and Related Structures, Physical Review Letters106, 176102 (2011).
 V. N. Strocov, H. I. Starnberg, P. O. Nilsson, H. E. Brauer, and L. J. Holle-boom, New Method for Absolute Band Structure Determination by Combin-ing Photoemission with Very-Low-Energy Electron Diffraction: Application to LayeredVSe2, Physical Review Letters 79, 467 (1997).
 J. Jobst, J. Kautz, D. Geelen, R. M. Tromp, and S. J. van der Molen,Nanoscale measurements of unoccupied band dispersion in few-layer graphene, Nature Communications6, 8926 (2015).
 J. B. Hannon, J. Sun, K. Pohl, and G. L. Kellogg,Origins of Nanoscale Het-erogeneity in Ultrathin Films, Physical Review Letters96, 246103 (2006).  J. Kautz, J. Jobst, C. Sorger, R. M. Tromp, H. B. Weber, and S. J. van der
 D. Geelen, A. Thete, O. Schaff, A. Kaiser, S. J. van der Molen, and R. Tromp,
Formation of a mixed ordered
termination on the surface of
We have investigated the surface termination of LaAlO3(001) at elevated
temper-atures by Low-Energy Electron Microscopy (LEEM). The terminating layer can be LaO or AlO2. The LaO surface shows a
5×√5 R26reconstruction which can be used as a signature for the LaO termination, while the AlO2 termination is
unre-constructed. We find that heating of as-delivered substrates in vacuum, or heating substrates which were previously annealed in air or oxygen, can lead to a recon-structed surface as observed in diffraction. However, the real-space image shows that the reconstructed areas only cover about a third of the surface and that the termination is actually an ordered mixture of the reconstructed LaO and the unre-constructed AlO2 terminations. This conclusion is supported by data from Atomic
Force Microscopy. We also demonstrate how the disordered mixture of both ter-minations changes to large LaO islands in the middle of the AlO2 terraces upon
A.J.H. van der Torren, S.J. van der Molen, J. Aarts
Formation of a mixed ordered termination on the LaAlO3
Much effort is currently directed to investigating the properties of interfaces be-tween perovskite oxides, in particular those of the ABO3 type, with particular
emphasis on the two-dimensional electron gas (2-DEG) which is formed between the insulators SrTiO3 (STO) and LaAlO3 (LAO)1. Of prime importance here is
control over and knowledge of the atomic termination layer of the surface on which the interface is prepared. For instance, in order to form the 2-DEG, it is well known that the STO surface has to be terminated with a TiO2 layer. Recipes exist for
the fabrication of different termination layers on the various substrates which are used in oxide research. Of recent interest are endeavors to fabricate mixed ordered terminations, which allow for the possibility to perform selective area growth.
In this study we focus on the surface of LaAlO3(001), which can be A-site
ter-minated with a layer of LaO or B-site terter-minated with a layer of AlO2. In the
literature, contradictory reports can be found on the issue of fabricating singly ter-minated surfaces. Kimet al.2use an 1100 ◦C annealing step in oxygen and find a predominantly AlO2termination, while Gunnarssonet al.3come to the conclusion
that the surface is doubly terminated when only annealed in oxygen. They report that etching the surface with HCl, followed by annealing in oxygen at the relatively low temperature of 800 ◦C leads to AlO
2termination3. Early work suggested that
also a complete A-site termination can be obtained even at 250◦C4,5, but this
finding could not be reproduced6. An LaO terminated surface was reported after
annealing at 700 ◦C in UHV using He atom scattering7, while similar annealing
was found to yield an AlO2 surface with 10 nm LaO islands8.
Extensive surface x-ray measurements were performed by Lanieret al. on surfaces which were prepared by annealing an LaAlO3 substrate between 1100 ◦C and
1500 ◦C in air9. Such surfaces show a clear√5×√5 R26 (RT5) reconstruction,
and it was concluded that it is the LaO layer which reconstructs, yielding a surface with one La vacancy per surface unit cell and stoichiometry (VLa4O5) (withV the
vacancy). We are not aware of a study of the occurrence of reconstructions on the AlO2-terminated surface, and as a working hypothesis we assume that it does not
Here we use Low-Energy Electron Microscopy (LEEM) to study the behavior of the LaAlO3 surface at high temperatures, an issue which is both relevant for surface
preparation and for growth. With the LEEM technique, we are able to discern different terminations in two ways. One is through the diffraction pattern when different reconstructions occur on the two terminations. By using apertures in the outgoing beams, LEEM also allows us to make a real space image of the occurrence of different reconstructions with high lateral resolution. The other way is to mea-sure the intensity of the diffraction spots (I), in particular of the specular beam, as function of the electron energy (V).
In this way we find for LaAlO3 that surfaces can be prepared with a single
termination of AlO2, but that high temperature treatments, presumably yielding
Figure 4.1: LEED pattern before a) and after b) annealing the sample at 1100 ◦C. The images
were taken at 17 eV and at 875◦C and 910◦C respectively. In (b), the diffraction spots of the
5×√5 R26 reconstruction are visible. Spots from two distinct domains are denoted with a green circle and a red square. The bright spot in the right top corner is due to secondary scattered electrons which are displaced from the center by dispersion in the system.
without reconstruction, and with differentIV characteristics. Complementing the LEEM data with room temperature AFM, we conclude that the annealing process leads to a mixed but ordered termination of both LaO and AlO2, with the LaO
termination occurring predominantly in the middle of terraces on the otherwise atomically flat surface.
The LEEM experiments were performed in the so-called ”Escher” setup, a state-of-the-art aberration-corrected LEEM facility at Leiden University10–13. In the
and accelerated again towards the objective lens. After passing the objective lens, they are deflected into the projection column and pass through a second magnetic prism deflecting the beam to an electrostatic mirror, a procedure which corrects for chromatic aberration10. Coming back from the mirror the electrons re-enter
the projection column and form a real-space or reciprocal space image on the channelplate detector.
With this system, various imaging modes can be used. In the first place low energy electron diffraction (LEED) can be used to study the structure of the surface. Lateral variations in the structure can be imaged by placing an aperture in the diffraction plane around one of the diffraction spots. By changing the projector lenses to produce a real space image, we can then study which areas of the sample contribute to that diffraction condition. This is called dark-field imaging. For so called bright-field mode the aperture is placed around the zeroth order LEED spot. Here we can still have contrast between structures with different reflection intensities (given by the structure factor) at a given electron energy. By measuring the intensity of the diffracted beam as function of electron energy at the sample, the so-called IV-curve, a specific signature of the surface can be obtained14–16. Since theIV curve of a surface is determined by the precise positions of the atoms, contrast between reconstructed and non-reconstructed areas can also be found at certain energies in bright field mode. To determine which areas in bright field belong to which reconstruction, the dark-field images are used.
Experiments in the LEEM are performed in a vacuum of 10−9 mbar, and the
sample can be continuously heated up to 1300 ◦C. Images are acquired with an acquisition time of 250 ms (four images per second) by a 1280x1024 pixel CCD camera behind a channel plate detector. Switching within less than a second be-tween different magnifications and image modes results in fast real time imaging of changes in the surface morphology.
Atomic Force Microscopy was routinely used to characterize the surface to-pography. A special experiment was performed on two samples to compare the information of LEEM and AFM on the same area. For this, trenches were etched in the surface using electron beam lithography and Ar-ion etching. These trenches served as markers both in the light microscope attached to the AFM and in the photo-emission mode of the LEEM, both of which have a field of view of a few hundred micrometer.
Figure 4.2:LEED-IV curves taken from the (0,0) spots of the LEED patterns shown in Fig. 4.1,
before and after annealing the sample.
An issue which surfaced in the research described here but which may well be more general, was that the as-received samples did not all behave in exactly the same manner. In the first set of experiments, a diffraction pattern pointing to a surface reconstruction could be directly obtained by annealing in vacuum at high temper-atures, but several attempts to make an AlO2-terminated surface by annealing in
oxygen failed. With a different batch of substrates, this (B-site) termination could be prepared, but obtaining the (A-site) reconstructed surface was only possible for a part of the surface. This will be detailed below.
In Fig. 4.1a we show the diffraction pattern of an as-received sample, taken at 875 ◦C, which shows an unreconstructed surface. The sample was then annealed in-situ for about 7 hours at a temperature of 1100 ◦C and cooled to 910 ◦C. This
resulted in the diffraction pattern given in Fig. 4.1b. It has four extra spots deriving from a rotated square surface net indicative of the RT5 reconstruction. Moreover, as indicated in the figure, the extra spots are doubled due to the fact that there are two equivalent rotations of the reconstruction, and both types are formed as domains on the surface. Fig. 4.2 shows theIV curve of the (0,0) spot for the sur-face before and after annealing. They are quite similar, although the curve after annealing shows a more pronounced maximum at 18 V and an additional peak at 22 V.
a 1 µm
Figure 4.3:a) Multi dark field and b) bright field image of LaAlO3after annealing above 1070◦C.
The images were taken at 15 eV and 17.6 respectively, at a temperature of 890◦C. The dark field
image consists of the two images of the distinct RT5 domains, overlaid in green and red.
separately. This is shown in Fig. 4.3a, where the two RT5 domains are color-coded in red and green. Interestingly, the reconstruction does not fully cover the surface. Rather it forms in stripe-like patterns with a more or less random variation of the two rotations, covering no more than about a third of the surface. The larger frac-tion of the surface is therefore not reconstructed. The reconstrucfrac-tion can also be imaged in bright-field, by choosing the appropriate energy, as shown in Fig. 4.3b taken at 17.6 eV. The two types of rotation are now not distinguishable, but other-wise the image faithfully reproduces the areas where the reconstruction is present (bright) or absent (dark). By taking bright field images at different electron ener-gies, it is also possible to generateIV curves at all positions on the surface. Fig. 4.4 shows suchIV curves of the (0,0) beam, taken on either a reconstructed (bright) or unreconstructed (dark) area. They are quite different. The unreconstructed area shows peaks around 5 V, 9 V, 12 V and 18 V, plus a small maximum around 25 V. The one from a reconstructed area shows peaks around 10 V and 18 V and generally shows a higher intensity, which leads to the contrast seen in Fig. 4.3b taken at 17.6 V. Comparing these data to theIV curves in Fig. 4.2 emphasizes thatIV curves taken on surfaces with a mix of reconstructed areas are of limited value. In particular the curve after annealing represents some weighted average of the two curves in Fig. 4.4 but cannot be used as the characteristic of either one of the surface terminations.
Although difficult to see in Fig. 4.3b there are also thin black lines visible in the bright-field image, which are related to and localized at step edges on the substrate. They can be seen to bend over roughly 90 o in the field of view, with the
Figure 4.4: IV curves taken from a selected area of the zero-order beam and taken from the reconstructed (bright) and unreconstructed (dark) areas on the surface. A circle containing 1264 pixels (equivalent to a diameter of about 100 nm) within a bright field image is averaged for every energy. Figure 4.3b is one of the bright field images out of this energy series.
visible, indicated by red arrows, and it is seen that the reconstructed area lies in the middle of the terrace, which is defined by the two steps. Fig. 4.5b shows an AFM image madeon the same area. The steps are sharp and clearly visible, but also the reconstructed area is visible in the AFM image, which therefore appears to be of different height. The cross-section from the AFM image, given in Fig. 4.5d shows that the steps around the reconstruction are about 0.35 nm high, corresponding to a full LaAlO3 unit cell. The steps bordering the reconstruction are smaller, only
about 0.1 nm, and the reconstructed areas lie deeper than the terrace on which they reside. The smaller steps can also be observed in the bright field image at the appropriate energy. Fig. 4.5c shows an image taken at 26.8 eV. This energy is chosen such that there is no contrast from the reconstruction, but there is (phase) contrast to observe the steps. The middle red arrow shows the right-hand step in the earlier image, but four extra steps appear (outer blue arrows) which border the reconstructed areas.
Most experiments in literature reporting the occurrence of the RT5 reconstruc-tion and/or a mixed terminareconstruc-tion were performed by extensive annealing of the LaAlO3sample in air or oxygen rather than in UHV as described above. We
200 nm c
a b d
Figure 4.5: a) Bright field image of LaAlO3 at 15.2 eV. Dark lines, indicated by red arrows,
are unit cell steps between substrate terraces. The bright area is the√5×√5 R26 reconstructed area. b) AFM image of same area. The thin white bar indicates the position of the cross section shown in d). This cross section is averaged over 7 lines in the image. c) Bright field image taken at 26.8 eV. The red arrow again indicates the step between the terraces while the blue arrows indicate the step between the terrace and the reconstruction. d) Height profile of the area given by the white line in b).
steps between the reconstructed and unreconstructed areas are clearly of half-unit cell height. This was less clear in Fig. 4.5 which could be caused by incomplete LaO termination. Looking closely at Fig. 4.5a again reveals numerous small dark spots within the bright area. Possibly the LaO termination is not fully developed and small AlO2islands still remain. Averaging such AlO2areas with the LaO areas
might result in an AFM height profile with less than half-unit cell steps.
The singly terminated surface
To further understand the difference between the reconstructed and unreconstructed areas we prepared a sample with a single terminated surface. As described in the introduction, how to prepare a single AlO2termination is not completely obvious.
Samples from two batches were annealed in various ways, in oxygen at atmospheric pressure as well as in air and vacuum. Some where etched in HCl as reported in Ref. 3, others where directly annealed as reported by Ref. 17. None of them led to the desired unit-cell-step and terrace structure as reported e.g. in Ref. 3, 17. In a third batch, we succeeded using a two step process. The sample was first annealed at 800◦C in UHV, followed by exposure to air after cooling down to room tem-perature. A subsequent anneal at 1000◦C in UHV resulted in an unreconstructed surface (not shown). An AFM image of this surface is presented in Fig. 4.7a. Single steps with a height of 0.4 nm are visible, and equally important, no half-size steps were found in Fig. 4.5d, suggesting the surface is singly terminated, and presumably by AlO2. A LEED-IV curve taken on this surface is shown in Fig. 4.8. Comparison
40.0 0.5 1.0 1.5 Distance (µm) 0.0
0.4 0.8 1.2
Figure 4.6: a) Bright field image at 9.2 eV and b) dark field images at 14 eV of an LaAlO3
sample annealed in air; c) AFM image of the same area. According to the AFM image, the reconstructed areas clearly lie lower than the surrounding terraces. d) Height profile along the cross-section drawn in c). Both unit cell steps and full-unit cell steps are present. The half-unit cell steps correspond with the reconstructed areas while the full-half-unit cell steps are between two unreconstructed terraces.
on the reconstructed sample shows them to be virtually identical. From this we conclude that also the unreconstructed part of such surface is AlO2 terminated.